Developed by Subcommittee: D06.92
WITHDRAWN, NO REPLACEMENT
This test method provides a quick, reliable means to measure the wet zero-span tensile strength of a specimen of sheeted material.
Formerly under the jurisdiction of Committee D06 on Paper and Paper Products, this test method was withdrawn in August 2009 due to insufficient committee interest in reviewing and revising the standard.
1.1 This test method provides a quick, reliable means to measure the wet zero-span tensile strength of a specimen of sheeted material.
1.2 In cases where fibers are to be tested prior to finished production of paper or paperboard, a random standard aggregate of pulp fibers, or handsheet, produced using a standardized procedure, such as, TAPPI T205 is required.
1.3 This test method requires specimens such as those described in 1.2.
1.4 While testing is possible on finished paper or paperboard, information on fiber quality from intermediate steps in the pulping or papermaking process, or both, is frequently more useful for improving finished paper and paperboard quality or improving fiber utilization of recycled fibers, or fibers subjected to new pulping, bleaching, or finishing processes (1, 2, 3, 4).
1.5 The modifications of this test method required for testing finished paper is straightforward; however, testing shall be done in the two principle directions of the sheet, as required in Test Method D829. The finished paper or paperboard will generally have nonrandom fiber orientation, resulting in different strength properties in the two principle directions of the finished sheet. Testing of sheets having a grammage greater than 100 g/m, which includes some paper materials described as paper and many paperboards, is difficult because of problems associated with clamping of individual fibers as the number of fibers per unit area increases.
1.6 Modifications such as those in 1.5 are not described in this test method. If modifications are made, they must be acknowledged and clearly described in the report as deviations from the standard procedure.
1.7 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety and health practices and determine the applicability of regulatory limitations prior to use.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
D586 Test Method for Ash in Pulp, Paper, and Paper Products
D828 Test Method for Tensile Properties of Paper and Paperboard Using Constant-Rate-of-Elongation Apparatus
D829 Test Methods for Wet Tensile Breaking Strength of Paper and Paper Products
D1193 Specification for Reagent Water
D1968 Terminology Relating to Paper and Paper Products
E122 Practice for Calculating Sample Size to Estimate, With a Specified Tolerable Error, the Average for Characteristic of a Lot or Process
TAPPI StandardsT220 Physical testing of pulp handsheets